IEC 62044-3 pdf download Cores made of soft magnetic materials – Measuring methods – Part 3: Magnetic properties at high excitation level
This standard provides measuring methods for power loss and amplitude permeability ofmagnetic cores forming the closed magnetic circuits intended for use at high excitation levelsin inductors,chokes,transformers and similar devices for power electronics applications.
The methods given in this standard can cover the measurement of magnetic properties forfrequencies ranging practically from d.c. to 10 MHz, and even possibly higher，for thecalorimetric and reflection methods. The applicability of the individual methods to specificfrequency ranges is dependent on the level of accuracy that is to be obtained.
The methods in this standard are basically the most suitable for sine-wave excitations. Otherperiodic waveforms can also be used; however，adequate accuracy can only be obtained ifthe measuring circuitry and instruments used are able to handle and process the amplitudesand phases of the signals involved within the frequency spectrum corresponding to the giveninduction and field strength waveforms with only slightly degraded accuracy.
NOTE lt may be necessary for some magnetically soft metallic materials to follow specific general principles,customary for these materials，related to the preparation of specimens and prescribed calculations. Theseprinciples are formulated in lEC 60404-8-6.
The following normative documents contain provisions which，through reference in this text,constitute provisions of this part of lEC 62044. For dated references，subsequentamendments to,or revisions of, any of these publications do not apply.However，parties toagreements based on this part of EC 62044 are encouraged to investigate the possibility ofapplying the most recent editions of the normative documents indicated below.For undatedreferences, the latest edition of the normative document referred to applies.Members of lECand lSO maintain registers of currently valid lnternational Standards.
IEC 60050(221):1990，International Electrotechnical Vocabulary (IEV) – Chapter 221:Magnetic materials and components
Amendment 1 (1993)
Amendment 2 (1999)
IEC 60205:1966,Calculation of the effective parameters of magnetic piece parts
IEC 60367-1:1982,Cores for inductors and transformers for telecommunications – Part 1:Measuring methods
IEC 60401:1993,Ferrite materials – Guide on the format of data appearing in manufacturers’catalogues of transformer and inductor cores
3 Terms, definitions and symbols
For the purposes of this International Standard, the following definitions apply in addition tothose of lEG 60050(221).
(effective) amplitude permeability (symbols: amplitude permeability: ua,effective amplitude permeability : uea)
magnetic permeability obtained from the peak value of the effective magnetic induction，ie，and the peak value of the magnetic field strength，He, at the stated value of either,when themagnetic induction and magnetic field vary periodically with time and with an average of zero,and the material is initially in a specified neutralized state